- 105 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about ' Simulations of 3D detectors' - kendall

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

G. Giacomini(a), G-F. Dalla Betta(b),C. Piemonte(a), M. Povoli(b)

(a) Silicon Radiation Sensors @ FBK, Trento

(b) University of Trento and INFN

- 3D sensors: properties, state-of-the-art and technology @ FBK
- TCAD simulations for 3D sensors: peculiarities
- Selected simulations :
- C-V depletion map
- SLIM edge
- Signals from test beam charge sharing
- Multiplication effect (?)

ADVANTAGES:

- Electrode distance and active substrate thickness decoupled:

- Low depletion voltage

- Short Collection distance

- Smaller trapping probability after irradiation

High radiation hardness

- Active edges:

- Dead area reduced up to few microns

from the edge

First proposed by S. Parker et. al.

in NIMA 395 (1997), 328

Best result:

66% of the original signal after

Fluence = 8.8x1015 cm-2 1-MeV neq.

@ 100 V

DISADVANTAGES:

- Non uniform response due to electrodes
- Complicated technology
- Higher capacitance (X3) with respect to planar

C. Da Via et. al.: NIMA 604 (2009) 504

~ 200-mm P-type substrate, n-junction columns insulated by p-spray

NOT FULL PASSING COLUMNS

- fabrication process reasonably simple
- proved good performance up to irradiation fuence

of 1015 neq/cm2 (even with non optimized gap “d”)

but

- column depth difficult to control and to reproduce

- insufficient performance after very large irradiation fluences if “d” is too large

n+ col

p-spray

p+ col

FULL PASSING COLUMNS

- Column depth = wafer thickness
- More complicated process

back patterned

From G.-F. Dalla Betta, IEEE NSS 2010, N15-3

Simulations presented are performed with Synopsis Sentaurus

(former ISE-TCAD) 1D, 2D and 3D simulator

solving physical equations (Poisson, drift, diffusion, …)

Static and dynamics measurements

Wafer layout and fabrication

Process and device simulation

Interpretation of measurements

with simulations

Simulation for understanding the properties of different kind of 3D sensors have been the subject of many papers:

- Parker et al.: “3D – A proposed new architecture for solid-state radiation detectors”

NIM A395 (1997) 328-343

- Piemonte et al.: “Development of 3D detectors featuring columnar electrodes of the same doping type” NIMA 541 (2008) 441
- Zoboli et al.: “Double-Sided, Double-Type-Column 3-D Detectors: Design, Fabrication, and Technology Evaluation” TNS 55 (2008) 2775
- Pennicard et al.: “Simulations of radiation-damaged 3D detectors for the Super-LHC”

NIM A 592 (2008) 16–25

For the different technologies, we studied both static

(I-V and C-V) and dynamic behavior (signals from optical and high-energy particles).

Peculiarity of 3D detector simulations

For a 3D detector, we must use 3D simulations, since properties varies with depth.

high number of nodes, long CPU time, …

On the other hand, structures may show regular pattern and the elementary cell can be quite small.

Example of 3D layout

Simulated structure = elementary cell

Upper surface

80 mm

Bottom surface

METAL GRID

p+ column

n+ column

Capacitance vs Vbias of an array of n - columns vs p - columns (back) of a 3D diode.

C-V curve does not saturate

for Vbias > Vdepl, like in a standard

planar Diode (1D approx),

To understand this effect we simulate:

- elementary cell.
- p-spray profile measured with SIMS and inserted in simulation.

From G.-F. Dalla Betta, IEEE NSS 2010, N15-3

Capacitance vs Vbias of an array of n+columns vs p+columns (back) of a 3D diode.

C-V curve does not saturate

for Vbias > Vdepl, like in a standard

planar Diode (1D approx),

To understand this effect we simulate:

- elementary cell.
- p-spray profile measured with SIMS and inserted in simulation.

From G.-F. Dalla Betta, IEEE NSS 2010, N15-3

Hole concentration vs Vbias

1V

2V

3V

4V

6V= Vdepletion

8V

10V

- At mid-substrate, (hole) depletion already @ Vbias = 6 V.
- Important capacitance contribution from p-spray

which is slowly depleting also at higher voltages.

Problem:

ATLAS IBL requires a max. dead layer of 450 mm along Z

for FE-I4 read-out.

50 mm

p (ohmic) columns

Standard Active edge difficult to implement because of support wafer

SLIM EDGE

- Multiple Ohmic (p-col.) fence

termination

- Dead area can be as low

as~ 200 mm

250 mm

200 mm

SCRIBE LINE

Does it work?

n (junction) columns

From G. Giacomini, 6th “Trento”

WS on 3D and p-type detectors, March 2011

The scribe line is simulated as a low-t region:

if depletion region touches it HIGH current!!

80 mm

Vbias = 30 V

p+ (ohmic) columns

Hole density (cm-3)

SLICE AT Y = 100 mm

80 mm

Scribe line:

Very Low t

Domain of

simulation

Vbias = 30 V

250 mm

n+ (junction)

columns

SCRIBE LINE

Even for Vbias >> Vdepl, depletion region hardly extends beyond second p-col row.

5th cut

Experimentally, it works:

Dicing away one row at a time and measuring the I-V,

It is shown that one row of ohmic holes is sufficient to “stop” the depletion region

3th cut

6th cut

40 mm

1st cut

p+ (ohmic)

columns

n+ (junction)

columns

Example 3. Signal from irradiated devices

Old FBK 3D sensor, not full passing columns

proton irradiated @ 1e15 neq/cm2

Collimated

Sr source

Qmean (fC))

Vbias (V)

C. Gallrap et al., "Characterisation of irradiated FBK sensors".

ATLAS 3D Sensor General Meeting, CERN, October 26, 2010.

We want to reproduce this “not intuitive” trend:

3D is “ideal” only in the columnar overlapping, while only a simulation can predict the collection of electrons generated below the column fluence dependent

Signal from irradiated devices

X

Bulk simulated according to “Perugia” model:

Petasecca TNS 53 (2006) 2971;

Pennicard NIM A 592 (2008) 16–25

N-column 2

To simulate the charge sharing:

double the elementary cell

m.i.p. crossing the bulk simulated with

uniform charge release (80 pairs/mm)

and with different track angles

N-column1

Y

z

P-column

Signal from irradiated devices

Column N1- signals

Column N2- signals

Integrals of currents ( = total collected Charge)

saturate before 20 ns (no ballistic deficit for ATLAS ROC)

and at a value exceeding the threshold of 3200 e- (0.5 fC) (ATLAS threshold)

Signal from irradiated devices

Simulating Cluster size 1 vs Bias voltage and

Simulating Cluster size 2 vs Bias voltage (for few impinging points) and

weighting the simulated results with geometrical/experimental considerations,

we get a simulated curve of the total charge vs Vbias, which fits well the irradiation experiment results.

Example 4. Multiplication effects work in progress!

In an irradiated p-on-n strip sensor (F= 1e15 neq/cm2), already at ~ 150 V,

CCE vs V plots shows an anomalous increase of IV and CCE-V.

It is believed that this effect comes from impact ionization

A. Zoboli, IEEE NSS 2008, N34-4

Multiplication effects work in progress!

Simulating multiplication with:

- impact ON

- effective bulk doping/oxide charge

no multiplication

- impact ON and

- traps from “Perugia” model

MULTIPLICATION close to the measured one

60

irradiated – F=1e15 neq

strip sensor p-on-n

charge

50

Simul. Leakage

Simul. Charge W traps

Simul. Charge W/o traps

Measured Charge

40

Current (mA)

Collected Charge (fC)

F = 1e15 neq/cm2

30

20

p-col

10

Vbias

n-substrate

n-col

CONCLUSIONS

Simulations of 3D are fundamental

because of the complexity of the device.

Different geometries & different Models must be chosen according to the simulation

We showed that simulations are useful both at the design

stage as well as to understand peculiar effects.

Download Presentation

Connecting to Server..